Microstructure and mechanical properties of as-quenched Mg ... Microstructure and mechanical...
Embed Size (px)
Transcript of Microstructure and mechanical properties of as-quenched Mg ... Microstructure and mechanical...
Microstructure and mechanical properties of as-quenched Mg-Gd-Zr alloys
HU Yao-bo1, 2, DENG Juan1, 2, ZHAO Chong1, 2, WANG Jing-feng1, 2, PAN Fu-sheng1, 2
1. College of Materials Science and Engineering, Chongqing University, Chongqing 400044, China;
2. National Engineering Research Center for Magnesium Alloys, Chongqing University, Chongqing 400044, China
Received 23 September 2010; accepted 25 December 2010
Abstract: Mg-xGd-0.6Zr (x=2, 4, 6, mass fraction) alloys were prepared by semi-continuous casting process. The effects of Gd content on the microstructures and mechanical properties of Mg-xGd-0.6Zr alloys were studied and the solid solution treatment process of Mg-6Gd-0.6Zr alloys was optimized. The microstructures and mechanical properties of all the studied alloys were analyzed by optical microscope, X-ray diffraction, scanning electron microscope equipped with energy dispersive spectroscope and micro-hardness tester. The results show that the grain size slightly decreases with increasing Gd content and there is a close linear relationship between Gd content and micro-hardness of Mg-xGd-0.6Zr alloys. The second phases Mg2Gd and Mg3Gd formed due to non-equilibrium solidification during the casting process can be transformed into equilibrium phase Mg5.05Gd which can dissolve into α-Mg solid solution phase at solution temperature of 460 °C. The optimized solid solution treatment of Mg-6Gd-0.6Zr alloy is (300 °C, 6 h) + (460 °C, 10 h). Key words: magnesium alloys; gadolinium; zirconium; microstructure; hardness; heat treatment 1 Introduction
Magnesium alloys have been intensively investigated in recent years due to their low density, high damping and excellent environmental protection performance. But the low strength of magnesium alloys limits their extensive applications[1−3]. Rare-earths- containing magnesium alloys reveal outstanding mechanical properties at room and elevated temperatures, especially Mg-Gd series alloys which provide excellent cast performance, mechanical properties and corrosion resistance. On the basis of previous investigations, magnesium alloys containing over 10% (mass fraction) Gd show excellent mechanical properties at room and elevate temperatures[5−8]. The strength of Mg-Gd series alloys increases greatly with increasing Gd content, and the change of elongation is contradictory due to their obvious precipitation hardening[9−10]. However, precipitation hardening and solid solution strengthening are two major strengthening mechanisms by the addition of Gd to Mg alloys[11−17]. Few researches were conducted on those alloys containing less than 10% Gd, especially the effect of Gd content less than 10% on solid
solution strengthening of Mg-Gd-Zr alloys. The aim of this work is to explore the effect of Gd content on the microstructure and mechanical properties of Mg-xGd-0.6Zr alloys and optimize the solid solution process of Mg-6Gd-0.6Zr. 2 Experimental
The elements of Mg, Gd and Zr in the experimental alloys were supplied in the form of pure Mg (99.8%, mass fraction), Mg-24.51%Gd and Mg-27.85%Zr master alloys. The Mg-xGd-0.6Zr (x=2, 4, 6 mass fraction) alloys were prepared by semi-continuous casting process. The actual compositions of the alloys were determined by XRD−1800 CCDE X-ray fluorescence spectrometer, as shown in Table 1.
As-cast GKx(x=2, 4, 6) alloys were held at 400 °C for 6 h, and at 500 °C for 10 h, then quenched into water to obtain as-quenched GKx alloys. DSC curve of as-cast GK6 alloy was used to determine the solid solution temperature range. GK6 alloy was held at 300 °C for 6 h, and held at 400, 420, 440, 460, 480 and 500 °C for 10 h, respectively, then quenched into water. The effect of Gd content on the microstructures and micro-hardness of
Foundation item: Project (50725413) supported by the National Natural Science Foundation of China; Project (CDJZR10130020) supported by the
Fundamental Research Funds for the Central Universities, China Corresponding author: HU Yao-bo; Tel:+86-13436117593; E-mail:email@example.com DOI: 10.1016/S1003-6326(11)60773-5
HU Yao-bo, et al/Trans. Nonferrous Met. Soc. China 21(2011) 732−738 733
Table 1 Nominal and actual compositions of Mg-Gd-Zr alloys
Actual mass fraction/% Actual molar fraction/% Alloy No. Nominal composition
Gd Zr Mg Gd Zr Mg
GK2 Mg-2Gd-0.6Zr 1.681 0.333 Bal. 0.320 0.102 Bal.
GK4 Mg-4Gd-0.6Zr 3.845 0.480 Bal. 0.747 0.149 Bal.
GK6 Mg-6Gd-0.6Zr 6.501 0.380 Bal. 1.291 0.121 Bal.
Mg-xGd-0.6Zr alloys were studied and the solid solution treatment process of Mg-6Gd- 0.6Zr alloys was optimized. The microstructures and mechanical properties of the alloys were analyzed by optical microscope (OM, MDS produced by OPTEC Company), X-ray diffractometer (XRD, D/max−1200, Cu, 40 kV, 250 mA, 4(°)/min, 10°−90°), scanning electron microscope (SEM, VEGA Ⅱ LMU) equipped with energy dispersive spectroscope (EDS, INCA Energy 350) and micro-hardness tester (HXL−1000AY). In micro-hardness test the load and holding time were 0.49 N and 10 s, respectively. 3 Results and discussion 3.1 Effects of Gd content on microstructures and
mechanical properties of as-quenched Mg-xGd- 0.6Zr alloys Figure 1 shows the optical microstructures of
as-quenched GKx alloys. The mean grain size was measured by linear intercept method. The grain sizes are 54, 48.5, 40.3 μm for GK2, GK4 and GK6 alloys, respectively. With the increase of Gd content, the grain size decreases. According to the Mg-Zr and Mg-Gd phase diagram, it is known that the equilibrium solid solubilities of Zr and Gd in Mg are 0.6% and 22%(mass fraction) at 500 °C. So Zr is hardly solution treated into Mg. Intragranular black phase could be Zr-rich phase in Zr-containing Mg alloys, which is not characterized in this work. From the optical microstructure of the alloys, it is seen that there is no phase existing along the grain interface of excluded GK6 alloy, as shown in Fig.1. Figure 2 shows SEM image of as-quenched GK6 alloy. Some white areas appear in matrix along the gain boundary. There is no obvious element-rich phase, as shown in Fig.3. The distribution of Gd in white area is more than that in other matrix.
The XRD patterns (Fig.4) of GKx alloys show that no new phase emerges with increasing the Gd content. α-Mg solid solution phase is the main phase. So Gd has been dissolved into the α-Mg matrix. From the precious EDS results, there is some Zr in the alloys. But the Zr peaks are not marked in Fig.4 because the hexagonal crystal structure of Zr is the same as that of Mg and their peaks coincide with Mg peak. Figure 5 shows Mg peak shifting of as-quenched GKx alloys due
Fig.1 Optical microstructures of as-quenched GK alloys: (a) GK2; (b) GK4; (c) GK6 to the increase of Gd content.
Figure 6 shows the variation of micro-hardness with Gd content in the as-quenched Mg-Gd-Zr alloys. It seems that the micro-hardness increases monotonically with the increase of Gd content. The hardness (H) is fitted to the Gd content (molar fraction) as
H = 40.16 + 9.30x(Gd) (x(Gd)=0.32−1.29) (1)
where x(Gd) is the Gd molar fraction. Eq.(1) and Fig.6 indicate a near linear increase of hardness with solute
HU Yao-bo, et al/Trans. Nonferrous Met. Soc. China 21(2011) 732−738 734
Fig.2 SEM image of as-quenched GK6 alloy concentration, which is very close to the results of Mg-Gd binary alloys. It was reported that the relationship between micro-hardness of Mg-Gd alloys and Gd content in Mg can be expressed as: H=37+14x(Gd) (x(Gd)=0.49−3.63) (2)
3.2 DSC analyses of as-cast Mg-6Gd-0.6Zr alloy Figure 7 shows the DSC curve of GK6 alloy. There
are three peaks in the curve. The peak at 648 °C should be attributed to Mg melting process, which is an endothermic reaction. From XRD patterns of as-cast GK6 alloys shown in Fig.8, the second phases in as-cast GK6 alloy disappear after solid solution treatment. So in the former two peaks, at least one or two should be the second phases heating reaction peaks. It can be seen that the broadening of peaks is obvious. Maybe a large of residual stress exists in the alloys due to the non-equilibrium solidification during the casting process, or hardening in the intercepting procedure of the studied sample. When the alloys are heated to certain temperature, a large of residual stress is released, which is an exothermic reaction, and leads to partly offset the endothermic peak required by heating reaction of the second phases to make these two peaks broaden and weaken.
There are a large number of Mg2Gd, Mg3Gd phases in as-cast GK6 alloy, but peaks of the new phase
Fig.3 Microstructure (a) and elements distribution of Mg (b), Gd (c) and Zr (d) in as-quenched GK6 alloys
HU Yao-bo, et al/Trans. Nonferrous Met. Soc. China 21(2011) 732−738 735
Fig.4 XRD patterns of as-quenched GKx alloys
Fig.5 XRD peak shifting of as-quenched GKx due to addition of Gd
Fig.6 Relationship between hardness and Gd content in as-quenched Mg-Gd-Zr alloys Mg5.05Gd appear at low angles and the peaks of Mg2Gd in the 2θ range of 28−29° become weaker after solution treatment at 400 °C. According to the Mg-Gd ph